Specification of an Operator for the Design of Architectural Forms: “Pleating”
During the creative phase, the architect introduces hypotheses and validates them by trying out various adjustments during the process of conception. The use of existing CAD tools during the conception phase is not compatible with the iterative aspect of this process. So the challenge is to define a model that takes into account the entire creative process in a trial and error framework during the conceptual phase. In this article we will define the “pleating” operator.
Specification and Implementation of a Folding Parametric Operator to Assist Architectural Conception at the Drafting Stage
In the early stage of creation, the architect tests his work hypotheses by making many adjustments while designing. During the sketching phase, the existing modeling tools are not compatible with the iterative nature of this process. So the challenge lies in the definition of a model which will allow the whole creative process with its various trying and going back during the phase of conception. We will illustrate this model by implementing a parametric operator allowing the action of folding. Its parametric specificity will enable the architect, in the design phase, to make the numerous moves and returns required to obtain an optimal shape.
Determination of Optimal Ball-Burnishing Parameters for Plastic Injection Moulding Steel
The objective of this study is to determine the optimal plane ball-burnishing parameters for plastic injection moulding steel PDS5 on a machining centre by utilising the Taguchi’s orthogonal array method. The design and manufacture of a burnishing tool are described. Four burnishing parameters, namely the ball material, burnishing speed, burnishing force and feed, were selected as the experimental factors in Taguchi’s design of experiments to determine the optimal burnishing parameters which have the dominant influence on surface roughness. The optimal burnishing parameters were found after carrying out the experiments specified by Taguchi’s L18 orthogonal table, by the analysis of variation, and by a full factorial experiment. The optimal plane burnishing parameters for the plastic injection moulding steel PDS5 were a combination of a tungsten carbide ball, a burnishing speed of 200 mm/min, a burnishing force of 300 N and a feed of 40 μm. The surface roughness Ra of the specimen can be improved from about 1 μm to 0.07 μm by using the optimal burnishing parameters for plane burnishing.